Journal of Molecular Catalysis A: Chemical 173 (2001) 275286
Poisoning and deactivation of palladium catalystsPeter Albers a, , Jrg Pietsch b , Stewart F. Parker ca
Infracor GmbH, Degussa-Hls Group, Department of Physical Chemistry, P.O. Box 1345, D-63403 Hanau, Germany b Degussa-Hls AG, Silica, Silanes & Catalysts, P.O. Box 1345, D-63403 Hanau, Germany c ISIS Facility, Rutherford Appleton Laboratory, Chilton, Didcot, Oxfordshire, OX11 0QX, UK Received 23 August 2000; received in revised form 20 October 2000; accepted 26 October 2000
Abstract Some of the major causes for deactivation and premature degradation of palladium catalysts are briey summarised. These include particle growth for various reasons, coke deposition and coke transformation, the inuence of the support material on long term stability and modications at the palladium surface itself such as valency changes or the formation of simple but stable molecular surface species. In addition, variations of physical properties as well as chemical poisoning, corrosion and leaching are discussed. In spite of the large body of literature concerning the common phenomenon catalyst deactivation specic information accessible for the various kinds of palladium catalysts being used worldwide is still quite limited. There is a serious need for future studies on properties of palladium-based catalytic systems regarding, for example, the interactions between carbon, hydrogen and supported palladium as a ternary system. Observations on different deactivation processes on Pd/SiO2 catalysts occuring under industrial conditions are compiled. It was tried to roughly differentiate between different degrees of coking and coke transformation in mainly thermally or purely catalytically driven catalyst coking on the one hand and of moderate or enhanced corrosion phenomena or changes of the properties of the palladium itself on the other. 2001 Elsevier Science B.V. All rights reserved.Keywords: Palladium catalysts; Catalyst deactivation; Palladium; Hydrogen; Carbon; Hydrogenation; Oxidation; Sintering; Agglomeration; Coking; Poisoning; Leaching
1. Introduction Uncontrolled and accidental poisoning or deactivation of palladium catalysts by various mechanisms can be a considerable nancial burden in chemical industry and is still on focus of academic as well as technological research. Some typical large scale applications of palladium catalysts are their use in the hydrogenation of organic ne chemicals, aromatic hydrogenations, Corresponding author. Tel.: +49-6181-592934; fax: +49-6181-592021. E-mail addresses: [email protected], [email protected] (P. Albers).
petroleum rening, the selective hydrogenation of acetylene to ethylene, the production of acetaldehyde by oxidation of ethene, the production of vinyl-acetate and, to an increasing extent, the use in different kinds of automotive exhaust gas catalysts [1,2]. As a result of the great economic relevance of palladium-based catalysts in these and related elds of chemical technology many investigations have been performed to study the physico-chemical properties of these materials in more detail and to reveal the various reasons for loss of activity or selectivity under unfavourable or irregular operation conditions. A better understanding of deactivation processes is essential for improving and optimising
1381-1169/01/$ see front matter 2001 Elsevier Science B.V. All rights reserved. PII: S 1 3 8 1 - 1 1 6 9 ( 0 1 ) 0 0 1 5 4 - 6
P. Albers et al. / Journal of Molecular Catalysis A: Chemical 173 (2001) 275286
process conditions, the catalysts themselves and for circumventing premature catalyst degradation in order to minimise additional costs. Conversely, controlled poisoning of palladium-based catalytic systems can have a benecial impact on performance. A prominent example is the use of lead compounds in the production of the Lindlar catalyst to improve and to ne-tune its properties such as the selectivity in the hydrogenation of CC to C=C bonds by blocking certain active sites [3,4]. In the present contribution, some of the most important reasons for the deactivation of palladium catalysts are sketched. A few examples and references were selected from the large body of existing literature on catalyst deactivation. They are focused predominantly on some recent and typical studies and observations including own work. A complete review addressing all different aspects of catalyst deactivation is beyond the scope of this short summary. Additional details and related references are accessible from authoritative surveys and proceedings (e.g. , and the literature cited therein).
2. Typical reasons for deactivation of palladium catalysts 2.1. Crystallite growth/sintering/agglomeration Morphological changes of palladium entities due to particle growth by different processes including sintering and agglomeration  are a major cause for a decrease of acitivity down to uneconomic levels or even complete deactivation of palladium catalysts. It has been observed that under the inuence of hydrogen particle growth of nely dispersed, unsupported palladium may occur even at temperatures as low as 330 K [11,12]. The various parameters governing particle growth phenomena have to be considered already during the rst steps of the preparation of palladium catalysts. Unfavourable and undesired effects may be suppressed by means of adequate impregnation agents and procedures, by controlled temperature and by the use of suitable support materials . An impact of the properties of the metal precursor as well as the support on the nal palladium dispersion obtained under identical preparation conditions was observed .
Conditioning treatments of the support materials by purication and by surface modication are well established as useful procedures especially in the eld of carbonaceous catalyst supports. Some examples are the treatments with oxidising agents such as hydrogen peroxide or by using acids the remove ashes and contaminants. For activated carbons or carbon blacks the cleaning and surface conditioning leads (e.g.) to the generation of surface functional groups and to an increasing accessability of other relevant sites including aromatic/graphitic structures and sites with few vicinal hydrogen atoms down to non-conjugated double bonds or vinylic/allylic entities. This can be of paramount inuence on the precious metal dispersion to be obtained in the nal Pd/C catalyst which are used (e.g.) in hydrogenation reactions . The ne structure of the carbon support materials [19,20], their purity, their surface chemistry and, therefore, the precious metal/support interactions have to be examined and optimised [1518,20] to establish adequate preparation conditions to achieve the best performance possible for the given application of the palladium catalyst. Regarding the stability of the palladium dispersion during reduction treatments the selection of suitable support materials is of great importance as well. Under a given set of conditions variations of precious metal dispersion and the loss of active area of a palladium catalyst with increasing temperature may be enhanced in the case of rather inert support materials compared to SiO2 or Al2 O3 [21,22]. This is also the case under the actual operation conditions of supported palladium catalysts: an inuence of the support on the stability of particle size was observed. Pd/TiO2 catalysts showed sintering at 500 C under the inuence of hydrogen whereas Pd/Al2 O3 catalysts were found to be more resistant under the same conditions . The Pd-based catalysts were identied as the most efcient ones for the catalytic combustion of methane to carbon dioxide and water. Also in these applications it was found that the tendency to sintering and poisoning and the thermal stability is dependent on the support . Considering the long term stability of the Pd-dispersion, again, interdependencies between support material and the resistance of the nal Pd-catalysts against catalyst deactivation were also found for other support materials such as ZrO2 , MgO, SiO2 /AlPO4 [25,26] or for ternary systems .
P. Albers et al. / Journal of Molecular Catalysis A: Chemical 173 (2001) 275286
Not only modication of the support but also of the precious metal component may be helpful: addition of (e.g.) Pt was shown to be effective in preventing catalyst deactivation by improving the heat resistance and the dispersion of supported oxidised palladium particles . Here, nely dispersed Pt crystallites, tightly attached to the support surface, were found to serve as anchoring sites for Pd. In the selective catalytic reduction of NOx by methane on Pd/zeolite catalysts a pronounced loss of acitivity was observed depending on the presence of water vapour. Formation of palladium oxide was detected and it was concluded that the tendency towards Pd-agglomeration was promoted by water . In addition to particle growth effects, valency changes between PdOx and metallic Pd may simultaneously be of prominent relevance . This illustrates that several positive or detrimental inuences could act together and might affect the degree and the stability of the dispersion of palladium particles including changes of the chemical valency in oxidation of particle surfaces on the one hand or the formation of palladium hydride on the other (Section 2.2.2). In addition to variations of the particle size a critical enhancement of the physical or chemical interactions between palladium and organic reactants, intermediates, by-products or degradation products, ending with signicant catalyst coking, can be of importance. The inuence of feed ratios during the operation of Pd/activated carbon catalysts that are deactivated by means of sintering or by coking has been revealed . 2.2. Inuenc